# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_lbsbo
_database_code_depnum_ccdc_archive 'CCDC 1911522'
loop_
_audit_author_name
_audit_author_address
'Xianghe Meng'
;Technical Institute of Physics and Chemistry
China
;
_audit_update_record             
;
2019-04-22 deposited with the CCDC.	2019-06-17 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'B8 Ba4 Li3 O22 Sc3'
_chemical_formula_weight         1143.54

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sc Sc 0.2519 0.3716 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   9.7959(3)
_cell_length_b                   10.2519(2)
_cell_length_c                   11.5878(3)
_cell_angle_alpha                85.069(2)
_cell_angle_beta                 68.734(2)
_cell_angle_gamma                62.795(2)
_cell_volume                     960.02(5)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    10811
_cell_measurement_theta_min      3.4850
_cell_measurement_theta_max      26.3510

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.956
_exptl_crystal_F_000             1024
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_absorpt_coefficient_mu    9.178
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.49321
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'XtaLAB Synergy, Dualflex, HyPix'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            25620
_diffrn_reflns_av_unetI/netI     0.0232
_diffrn_reflns_av_R_equivalents  0.0404
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_theta_min         2.794
_diffrn_reflns_theta_max         26.369
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_point_group_measured_fraction_full 0.998
_reflns_number_total             3921
_reflns_number_gt                3506
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0204P)²+1.0562P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         3921
_refine_ls_number_parameters     361
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0229
_refine_ls_R_factor_gt           0.0196
_refine_ls_wR_factor_ref         0.0509
_refine_ls_wR_factor_gt          0.0490
_refine_ls_goodness_of_fit_ref   1.066
_refine_ls_restrained_S_all      1.066
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1 Ba 0.12594(2) 0.80760(2) -0.14850(2) 0.00845(6) Uani 1 1 d . . . . .
Ba2 Ba 0.37961(2) 0.69832(2) 1.14932(2) 0.00847(6) Uani 1 1 d . . . . .
Ba3 Ba 0.32855(3) 0.35721(2) 0.55353(2) 0.00893(6) Uani 1 1 d . . . . .
Ba4 Ba 0.19285(3) 1.12431(2) 0.43844(2) 0.00955(6) Uani 1 1 d . . . . .
Sc1 Sc 0.23857(7) 0.74789(6) 0.50868(5) 0.00659(14) Uani 1 1 d . . . . .
Sc2 Sc 0.57523(8) 0.70243(7) 0.79199(6) 0.00534(13) Uani 1 1 d . . . . .
Sc3 Sc -0.07211(8) 0.78925(7) 0.21299(6) 0.00563(13) Uani 1 1 d . . . . .
O1 O 0.3537(3) 0.4507(3) 0.0847(2) 0.0129(5) Uani 1 1 d . . . . .
O2 O 0.1586(3) 1.0539(3) 0.9051(2) 0.0159(6) Uani 1 1 d . . . . .
O3 O -0.0219(3) 1.1239(3) 0.3434(2) 0.0094(5) Uani 1 1 d . . . . .
O4 O 0.1492(3) 0.8881(3) 0.3883(2) 0.0136(6) Uani 1 1 d . . . . .
O5 O 0.5115(3) 0.8513(3) 0.6578(2) 0.0110(5) Uani 1 1 d . . . . .
O6 O 0.0391(3) 0.9084(3) 0.2328(2) 0.0115(5) Uani 1 1 d . . . . .
O7 O 0.3076(3) 1.0871(3) 0.6404(2) 0.0099(5) Uani 1 1 d . . . . .
O8 O 0.3509(3) 0.8725(3) 0.5364(2) 0.0137(5) Uani 1 1 d . . . . .
O9 O 0.3707(3) 0.8399(3) 0.9412(2) 0.0104(5) Uani 1 1 d . . . . .
O10 O 0.5457(3) 0.3772(3) 0.6408(2) 0.0122(5) Uani 1 1 d . . . . .
O11 O 0.7968(3) 0.5804(3) 0.6400(2) 0.0109(5) Uani 1 1 d . . . . .
O12 O 0.4570(3) 0.5905(3) 0.7696(2) 0.0118(5) Uani 1 1 d . . . . .
O13 O 0.1316(3) 0.6650(3) 0.0608(2) 0.0102(5) Uani 1 1 d . . . . .
O14 O -0.0166(3) 0.6490(3) 0.3530(2) 0.0129(5) Uani 1 1 d . . . . .
O15 O 0.3279(3) 0.6035(3) 0.6288(2) 0.0151(6) Uani 1 1 d . . . . .
O16 O 0.1152(3) 0.6255(3) 0.4985(2) 0.0154(6) Uani 1 1 d . . . . .
O17 O 0.7234(3) 0.7923(3) 0.8095(2) 0.0115(5) Uani 1 1 d . . . . .
O18 O 0.2088(3) 0.3138(3) -0.1955(2) 0.0128(5) Uani 1 1 d . . . . .
O19 O 0.5808(3) 1.0559(3) 0.8212(2) 0.0179(6) Uani 1 1 d . . . . .
O20 O 0.0418(3) 0.5761(3) -0.1523(2) 0.0150(6) Uani 1 1 d . . . . .
O21 O 0.2489(3) 1.0770(3) 1.0568(2) 0.0124(5) Uani 1 1 d . . . . .
O22 O 0.2478(3) 0.4322(3) -0.0591(2) 0.0115(5) Uani 1 1 d . . . . .
B1 B 0.0538(4) 0.9727(4) 0.3221(3) 0.0055(7) Uani 1 1 d . . . . .
B2 B 0.3876(5) 0.9362(4) 0.6134(3) 0.0072(8) Uani 1 1 d . . . . .
B3 B 0.2656(5) 0.9840(4) 0.9643(4) 0.0082(8) Uani 1 1 d . . . . .
B4 B 0.2392(5) 0.5214(4) 0.0320(4) 0.0075(8) Uani 1 1 d . . . . .
B5 B 0.4448(5) 0.5251(4) 0.6785(3) 0.0068(8) Uani 1 1 d . . . . .
B6 B 0.1570(5) 0.4475(4) -0.1372(3) 0.0075(8) Uani 1 1 d . . . . .
B7 B 0.1012(5) 0.5670(4) 0.4030(4) 0.0076(8) Uani 1 1 d . . . . .
B8 B 0.6739(5) 0.9325(4) 0.8562(3) 0.0098(8) Uani 1 1 d . . . . .
Li1 Li -0.1855(9) 0.7123(8) -0.0482(7) 0.0279(17) Uani 1 1 d . . . . .
Li2 Li 0.4030(9) 1.1079(9) 0.7685(7) 0.0291(17) Uani 1 1 d . . . . .
Li3 Li -0.0604(11) 0.6012(9) -0.2768(8) 0.039(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba1 O3 2.716(2) 2_575 ?
Ba1 O13 2.727(2) . ?
Ba1 O12 2.811(2) 1_554 ?
Ba1 O2 2.831(3) 1_554 ?
Ba1 O20 2.854(3) . ?
Ba1 O15 2.897(3) 1_554 ?
Ba1 O6 2.897(2) 2_575 ?
Ba1 O2 3.018(3) 2_576 ?
Ba1 O21 3.070(3) 2_576 ?
Ba1 O9 3.088(3) 1_554 ?
Ba1 B5 3.217(4) 1_554 ?
Ba1 B1 3.222(4) 2_575 ?
Ba2 O9 2.714(2) . ?
Ba2 O10 2.738(2) 2_667 ?
Ba2 O19 2.785(3) 2_677 ?
Ba2 O1 2.850(3) 1_556 ?
Ba2 O6 2.855(2) 1_556 ?
Ba2 O1 2.904(3) 2_666 ?
Ba2 O12 2.914(2) 2_667 ?
Ba2 O4 2.988(2) 1_556 ?
Ba2 O22 3.035(2) 2_666 ?
Ba2 O13 3.114(3) 1_556 ?
Ba2 B1 3.199(4) 1_556 ?
Ba2 B5 3.207(4) 2_667 ?
Ba3 O15 2.737(3) . ?
Ba3 O10 2.754(3) . ?
Ba3 O16 2.784(2) . ?
Ba3 O8 2.789(3) 2_666 ?
Ba3 O18 2.795(2) 1_556 ?
Ba3 O11 2.824(2) 2_666 ?
Ba3 O5 2.841(2) 2_666 ?
Ba3 O14 2.878(3) 2_566 ?
Ba3 O7 2.935(2) 1_545 ?
Ba3 B5 3.126(4) . ?
Ba3 B2 3.158(4) 2_666 ?
Ba3 B7 3.228(4) . ?
Ba4 O3 2.707(3) . ?
Ba4 O8 2.733(2) . ?
Ba4 O4 2.784(3) . ?
Ba4 O16 2.804(3) 2_576 ?
Ba4 O5 2.823(3) 2_676 ?
Ba4 O17 2.858(2) 2_676 ?
Ba4 O7 2.872(2) . ?
Ba4 O14 2.914(3) 2_576 ?
Ba4 B1 3.117(4) . ?
Ba4 O11 3.121(2) 2_676 ?
Ba4 O19 3.123(3) 2_676 ?
Ba4 B8 3.180(4) 2_676 ?
Sc1 O4 2.041(2) . ?
Sc1 O15 2.059(2) . ?
Sc1 O10 2.088(2) 2_666 ?
Sc1 O3 2.090(2) 2_576 ?
Sc1 O8 2.135(3) . ?
Sc1 O16 2.137(3) . ?
Sc1 Ba4 3.6261(7) 2_576 ?
Sc1 Ba3 3.6607(7) 2_666 ?
Sc1 Ba1 3.7409(6) 1_556 ?
Sc1 Ba2 3.8802(6) 1_554 ?
Sc2 O12 2.052(3) . ?
Sc2 O9 2.078(2) . ?
Sc2 O1 2.080(2) 2_666 ?
Sc2 O17 2.114(3) . ?
Sc2 O11 2.122(2) . ?
Sc2 O5 2.136(2) . ?
Sc2 Li3 3.024(9) 1_656 ?
Sc2 Li1 3.511(8) 1_656 ?
Sc2 Ba4 3.7310(7) 2_676 ?
Sc2 Ba3 3.8012(6) 2_666 ?
Sc2 Ba1 3.8204(7) 1_556 ?
Sc3 O6 2.044(3) . ?
Sc3 O13 2.055(2) . ?
Sc3 O2 2.096(2) 2_576 ?
Sc3 O18 2.116(3) 2_565 ?
Sc3 O14 2.126(2) . ?
Sc3 O7 2.161(2) 2_576 ?
Sc3 Li2 2.841(8) 2_576 ?
Sc3 Ba3 3.7020(7) 2_566 ?
Sc3 Ba4 3.8328(7) 2_576 ?
Sc3 Ba2 3.8695(7) 1_554 ?
Sc3 Ba1 3.9598(7) 2_575 ?
O1 B4 1.354(5) . ?
O1 Sc2 2.080(2) 2_666 ?
O1 Ba2 2.850(3) 1_554 ?
O1 Ba2 2.904(2) 2_666 ?
O2 B3 1.354(5) . ?
O2 Sc3 2.096(2) 2_576 ?
O2 Li2 2.618(9) . ?
O2 Ba1 2.831(3) 1_556 ?
O2 Ba1 3.018(3) 2_576 ?
O3 B1 1.377(4) . ?
O3 Sc1 2.090(2) 2_576 ?
O3 Ba1 2.716(2) 2_575 ?
O4 B1 1.371(4) . ?
O4 Ba2 2.988(2) 1_554 ?
O4 Ba4 3.277(3) 2_576 ?
O5 B2 1.380(4) . ?
O5 Li2 2.595(9) . ?
O5 Ba4 2.823(3) 2_676 ?
O5 Ba3 2.841(2) 2_666 ?
O6 B1 1.356(5) . ?
O6 Ba2 2.855(2) 1_554 ?
O6 Ba1 2.897(2) 2_575 ?
O7 B2 1.379(4) . ?
O7 Li2 2.089(8) . ?
O7 Sc3 2.161(2) 2_576 ?
O7 Ba3 2.935(2) 1_565 ?
O8 B2 1.378(5) . ?
O8 Ba3 2.789(2) 2_666 ?
O9 B3 1.338(5) . ?
O9 Ba1 3.088(3) 1_556 ?
O10 B5 1.377(4) . ?
O10 Sc1 2.088(2) 2_666 ?
O10 Ba2 2.738(2) 2_667 ?
O11 B7 1.385(5) 2_666 ?
O11 Li3 2.054(9) 1_656 ?
O11 Ba3 2.824(2) 2_666 ?
O11 Ba4 3.121(2) 2_676 ?
O12 B5 1.365(5) . ?
O12 Ba1 2.811(2) 1_556 ?
O12 Ba2 2.914(2) 2_667 ?
O13 B4 1.341(5) . ?
O13 Ba2 3.114(3) 1_554 ?
O14 B7 1.375(5) . ?
O14 Li3 2.463(9) 2_565 ?
O14 Ba3 2.878(3) 2_566 ?
O14 Ba4 2.914(3) 2_576 ?
O15 B5 1.359(5) . ?
O15 Ba1 2.897(3) 1_556 ?
O16 B7 1.378(5) . ?
O16 Li3 2.614(10) 1_556 ?
O16 Ba4 2.804(2) 2_576 ?
O17 B8 1.377(5) . ?
O17 Li3 2.081(8) 1_656 ?
O17 Li1 2.085(8) 1_656 ?
O17 Ba4 2.858(2) 2_676 ?
O18 B6 1.366(5) . ?
O18 Li2 2.038(8) 1_544 ?
O18 Sc3 2.116(3) 2_565 ?
O18 Ba3 2.795(2) 1_554 ?
O19 B8 1.312(5) . ?
O19 Li2 1.886(8) . ?
O19 Ba2 2.785(3) 2_677 ?
O19 Ba4 3.123(3) 2_676 ?
O20 B6 1.336(5) . ?
O20 Li1 1.965(8) . ?
O20 Li3 1.975(8) . ?
O21 B3 1.412(5) . ?
O21 B8 1.438(5) 2_677 ?
O21 Li1 1.960(7) 2_576 ?
O21 Ba1 3.070(3) 2_576 ?
O22 B4 1.410(5) . ?
O22 B6 1.438(5) . ?
O22 Li1 2.018(7) 2_565 ?
O22 Ba2 3.035(2) 2_666 ?
B1 Ba2 3.199(4) 1_554 ?
B1 Ba1 3.222(4) 2_575 ?
B1 Ba4 3.374(3) 2_576 ?
B2 Li2 2.708(9) . ?
B2 Ba3 3.158(4) 2_666 ?
B3 Li2 2.725(9) . ?
B3 Ba1 3.288(4) 1_556 ?
B3 Ba1 3.344(4) 2_576 ?
B4 Li1 2.656(8) 2_565 ?
B4 Ba2 3.296(4) 2_666 ?
B4 Ba2 3.331(4) 1_554 ?
B5 Ba2 3.207(4) 2_667 ?
B5 Ba1 3.217(4) 1_556 ?
B5 Ba3 3.343(4) 2_666 ?
B6 Li1 2.606(8) 2_565 ?
B6 Ba3 3.362(4) 1_554 ?
B7 O11 1.385(5) 2_666 ?
B7 Li3 2.600(10) 2_565 ?
B7 Ba4 3.242(4) 2_576 ?
B8 O21 1.438(5) 2_677 ?
B8 Li1 2.460(8) 1_656 ?
B8 Ba4 3.180(4) 2_676 ?
Li1 O21 1.960(7) 2_576 ?
Li1 O22 2.018(7) 2_565 ?
Li1 O17 2.085(8) 1_454 ?
Li1 B8 2.460(8) 1_454 ?
Li1 Li3 2.589(12) . ?
Li1 B6 2.606(8) 2_565 ?
Li1 B4 2.656(8) 2_565 ?
Li1 Li2 3.297(12) 2_576 ?
Li1 Sc2 3.511(8) 1_454 ?
Li1 Ba2 4.103(8) 1_454 ?
Li2 O18 2.038(8) 1_566 ?
Li2 Sc3 2.841(8) 2_576 ?
Li2 Li1 3.297(12) 2_576 ?
Li2 Ba3 3.433(7) 1_565 ?
Li2 Ba4 3.545(8) 2_676 ?
Li2 Ba2 3.880(8) 2_677 ?
Li3 O11 2.054(9) 1_454 ?
Li3 O17 2.081(8) 1_454 ?
Li3 O14 2.463(9) 2_565 ?
Li3 B7 2.600(10) 2_565 ?
Li3 O16 2.614(10) 1_554 ?
Li3 Sc2 3.024(9) 1_454 ?
Li3 Ba4 3.260(8) 2_575 ?
Li3 Ba3 3.367(8) 1_554 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 Ba1 O13 149.37(8) 2_575 . ?
O3 Ba1 O12 109.73(7) 2_575 1_554 ?
O13 Ba1 O12 79.49(7) . 1_554 ?
O3 Ba1 O2 104.88(7) 2_575 1_554 ?
O13 Ba1 O2 101.78(7) . 1_554 ?
O12 Ba1 O2 100.57(8) 1_554 1_554 ?
O3 Ba1 O20 80.61(7) 2_575 . ?
O13 Ba1 O20 70.53(7) . . ?
O12 Ba1 O20 87.10(7) 1_554 . ?
O2 Ba1 O20 168.16(8) 1_554 . ?
O3 Ba1 O15 63.28(7) 2_575 1_554 ?
O13 Ba1 O15 111.44(7) . 1_554 ?
O12 Ba1 O15 48.89(7) 1_554 1_554 ?
O2 Ba1 O15 125.84(8) 1_554 1_554 ?
O20 Ba1 O15 65.97(8) . 1_554 ?
O3 Ba1 O6 49.77(7) 2_575 2_575 ?
O13 Ba1 O6 142.55(7) . 2_575 ?
O12 Ba1 O6 132.26(8) 1_554 2_575 ?
O2 Ba1 O6 58.77(7) 1_554 2_575 ?
O20 Ba1 O6 121.90(7) . 2_575 ?
O15 Ba1 O6 105.53(7) 1_554 2_575 ?
O3 Ba1 O2 111.13(7) 2_575 2_576 ?
O13 Ba1 O2 60.47(7) . 2_576 ?
O12 Ba1 O2 138.08(7) 1_554 2_576 ?
O2 Ba1 O2 77.69(9) 1_554 2_576 ?
O20 Ba1 O2 90.57(8) . 2_576 ?
O15 Ba1 O2 156.25(8) 1_554 2_576 ?
O6 Ba1 O2 83.14(7) 2_575 2_576 ?
O3 Ba1 O21 69.68(7) 2_575 2_576 ?
O13 Ba1 O21 89.79(7) . 2_576 ?
O12 Ba1 O21 155.37(7) 1_554 2_576 ?
O2 Ba1 O21 103.32(7) 1_554 2_576 ?
O20 Ba1 O21 68.37(7) . 2_576 ?
O15 Ba1 O21 117.83(7) 1_554 2_576 ?
O6 Ba1 O21 67.35(7) 2_575 2_576 ?
O2 Ba1 O21 44.53(7) 2_576 2_576 ?
O3 Ba1 O9 138.65(7) 2_575 1_554 ?
O13 Ba1 O9 71.70(7) . 1_554 ?
O12 Ba1 O9 60.51(7) 1_554 1_554 ?
O2 Ba1 O9 46.93(7) 1_554 1_554 ?
O20 Ba1 O9 133.78(7) . 1_554 ?
O15 Ba1 O9 105.49(7) 1_554 1_554 ?
O6 Ba1 O9 104.28(7) 2_575 1_554 ?
O2 Ba1 O9 93.29(7) 2_576 1_554 ?
O21 Ba1 O9 136.63(6) 2_576 1_554 ?
O3 Ba1 B5 88.12(8) 2_575 1_554 ?
O13 Ba1 B5 91.69(8) . 1_554 ?
O12 Ba1 B5 25.04(9) 1_554 1_554 ?
O2 Ba1 B5 119.58(9) 1_554 1_554 ?
O20 Ba1 B5 70.54(9) . 1_554 ?
O15 Ba1 B5 24.99(8) 1_554 1_554 ?
O6 Ba1 B5 125.52(8) 2_575 1_554 ?
O2 Ba1 B5 150.86(8) 2_576 1_554 ?
O21 Ba1 B5 135.71(9) 2_576 1_554 ?
O9 Ba1 B5 85.03(8) 1_554 1_554 ?
O3 Ba1 B1 24.99(9) 2_575 2_575 ?
O13 Ba1 B1 154.06(8) . 2_575 ?
O12 Ba1 B1 125.36(8) 1_554 2_575 ?
O2 Ba1 B1 82.29(8) 1_554 2_575 ?
O20 Ba1 B1 100.73(8) . 2_575 ?
O15 Ba1 B1 85.18(8) 1_554 2_575 ?
O6 Ba1 B1 24.88(8) 2_575 2_575 ?
O2 Ba1 B1 96.20(8) 2_576 2_575 ?
O21 Ba1 B1 64.48(8) 2_576 2_575 ?
O9 Ba1 B1 124.49(8) 1_554 2_575 ?
B5 Ba1 B1 108.73(10) 1_554 2_575 ?
O9 Ba2 O10 156.00(8) . 2_667 ?
O9 Ba2 O19 73.64(8) . 2_677 ?
O10 Ba2 O19 83.94(8) 2_667 2_677 ?
O9 Ba2 O1 99.27(7) . 1_556 ?
O10 Ba2 O1 102.61(7) 2_667 1_556 ?
O19 Ba2 O1 172.39(7) 2_677 1_556 ?
O9 Ba2 O6 79.98(7) . 1_556 ?
O10 Ba2 O6 106.00(7) 2_667 1_556 ?
O19 Ba2 O6 82.79(8) 2_677 1_556 ?
O1 Ba2 O6 98.89(7) 1_556 1_556 ?
O9 Ba2 O1 62.28(7) . 2_666 ?
O10 Ba2 O1 116.03(7) 2_667 2_666 ?
O19 Ba2 O1 102.22(8) 2_677 2_666 ?
O1 Ba2 O1 71.54(9) 1_556 2_666 ?
O6 Ba2 O1 137.95(7) 1_556 2_666 ?
O9 Ba2 O12 141.89(7) . 2_667 ?
O10 Ba2 O12 49.60(7) 2_667 2_667 ?
O19 Ba2 O12 125.85(7) 2_677 2_667 ?
O1 Ba2 O12 58.36(7) 1_556 2_667 ?
O6 Ba2 O12 130.16(8) 1_556 2_667 ?
O1 Ba2 O12 80.57(7) 2_666 2_667 ?
O9 Ba2 O4 114.82(7) . 1_556 ?
O10 Ba2 O4 60.78(7) 2_667 1_556 ?
O19 Ba2 O4 65.24(8) 2_677 1_556 ?
O1 Ba2 O4 121.26(8) 1_556 1_556 ?
O6 Ba2 O4 47.70(7) 1_556 1_556 ?
O1 Ba2 O4 166.88(7) 2_666 1_556 ?
O12 Ba2 O4 103.30(7) 2_667 1_556 ?
O9 Ba2 O22 91.93(7) . 2_666 ?
O10 Ba2 O22 74.97(7) 2_667 2_666 ?
O19 Ba2 O22 78.44(8) 2_677 2_666 ?
O1 Ba2 O22 99.36(7) 1_556 2_666 ?
O6 Ba2 O22 161.01(7) 1_556 2_666 ?
O1 Ba2 O22 45.88(7) 2_666 2_666 ?
O12 Ba2 O22 65.28(7) 2_667 2_666 ?
O4 Ba2 O22 124.07(7) 1_556 2_666 ?
O9 Ba2 O13 71.43(7) . 1_556 ?
O10 Ba2 O13 131.76(7) 2_667 1_556 ?
O19 Ba2 O13 131.01(7) 2_677 1_556 ?
O1 Ba2 O13 46.48(7) 1_556 1_556 ?
O6 Ba2 O13 58.28(7) 1_556 1_556 ?
O1 Ba2 O13 90.78(7) 2_666 1_556 ?
O12 Ba2 O13 102.68(7) 2_667 1_556 ?
O4 Ba2 O13 100.44(7) 1_556 1_556 ?
O22 Ba2 O13 135.22(6) 2_666 1_556 ?
O9 Ba2 B1 91.99(8) . 1_556 ?
O10 Ba2 B1 86.09(8) 2_667 1_556 ?
O19 Ba2 B1 65.04(9) 2_677 1_556 ?
O1 Ba2 B1 118.78(9) 1_556 1_556 ?
O6 Ba2 B1 25.07(9) 1_556 1_556 ?
O1 Ba2 B1 154.11(8) 2_666 1_556 ?
O12 Ba2 B1 125.30(8) 2_667 1_556 ?
O4 Ba2 B1 25.31(8) 1_556 1_556 ?
O22 Ba2 B1 140.42(8) 2_666 1_556 ?
O13 Ba2 B1 82.92(8) 1_556 1_556 ?
O9 Ba2 B5 155.14(8) . 2_667 ?
O10 Ba2 B5 25.23(8) 2_667 2_667 ?
O19 Ba2 B5 102.87(9) 2_677 2_667 ?
O1 Ba2 B5 82.37(8) 1_556 2_667 ?
O6 Ba2 B5 124.50(8) 1_556 2_667 ?
O1 Ba2 B5 95.45(8) 2_666 2_667 ?
O12 Ba2 B5 25.20(8) 2_667 2_667 ?
O4 Ba2 B5 84.23(8) 1_556 2_667 ?
O22 Ba2 B5 63.47(8) 2_666 2_667 ?
O13 Ba2 B5 122.88(8) 1_556 2_667 ?
B1 Ba2 B5 109.09(9) 1_556 2_667 ?
O15 Ba3 O10 50.99(7) . . ?
O15 Ba3 O16 63.61(7) . . ?
O10 Ba3 O16 113.69(7) . . ?
O15 Ba3 O8 110.31(8) . 2_666 ?
O10 Ba3 O8 64.79(7) . 2_666 ?
O16 Ba3 O8 143.37(8) . 2_666 ?
O15 Ba3 O18 87.85(8) . 1_556 ?
O10 Ba3 O18 77.71(7) . 1_556 ?
O16 Ba3 O18 111.88(7) . 1_556 ?
O8 Ba3 O18 103.62(7) 2_666 1_556 ?
O15 Ba3 O11 109.45(7) . 2_666 ?
O10 Ba3 O11 145.44(7) . 2_666 ?
O16 Ba3 O11 50.32(7) . 2_666 ?
O8 Ba3 O11 108.33(7) 2_666 2_666 ?
O18 Ba3 O11 134.71(7) 1_556 2_666 ?
O15 Ba3 O5 139.52(8) . 2_666 ?
O10 Ba3 O5 112.99(7) . 2_666 ?
O16 Ba3 O5 108.78(7) . 2_666 ?
O8 Ba3 O5 50.35(7) 2_666 2_666 ?
O18 Ba3 O5 128.34(7) 1_556 2_666 ?
O11 Ba3 O5 60.51(7) 2_666 2_666 ?
O15 Ba3 O14 116.07(8) . 2_566 ?
O10 Ba3 O14 139.63(7) . 2_566 ?
O16 Ba3 O14 76.39(7) . 2_566 ?
O8 Ba3 O14 130.39(7) 2_666 2_566 ?
O18 Ba3 O14 62.79(7) 1_556 2_566 ?
O11 Ba3 O14 72.09(7) 2_666 2_566 ?
O5 Ba3 O14 98.59(7) 2_666 2_566 ?
O15 Ba3 O7 142.78(7) . 1_545 ?
O10 Ba3 O7 105.95(7) . 1_545 ?
O16 Ba3 O7 134.89(7) . 1_545 ?
O8 Ba3 O7 73.38(7) 2_666 1_545 ?
O18 Ba3 O7 56.30(7) 1_556 1_545 ?
O11 Ba3 O7 103.76(7) 2_666 1_545 ?
O5 Ba3 O7 72.54(7) 2_666 1_545 ?
O14 Ba3 O7 59.32(7) 2_566 1_545 ?
O15 Ba3 B5 25.72(8) . . ?
O10 Ba3 B5 26.11(8) . . ?
O16 Ba3 B5 89.33(9) . . ?
O8 Ba3 B5 89.80(9) 2_666 . ?
O18 Ba3 B5 77.34(8) 1_556 . ?
O11 Ba3 B5 132.82(8) 2_666 . ?
O5 Ba3 B5 133.69(8) 2_666 . ?
O14 Ba3 B5 127.40(8) 2_566 . ?
O7 Ba3 B5 123.27(8) 1_545 . ?
O15 Ba3 B2 132.51(9) . 2_666 ?
O10 Ba3 B2 90.60(9) . 2_666 ?
O16 Ba3 B2 132.58(9) . 2_666 ?
O8 Ba3 B2 25.86(9) 2_666 2_666 ?
O18 Ba3 B2 112.83(8) 1_556 2_666 ?
O11 Ba3 B2 86.30(9) 2_666 2_666 ?
O5 Ba3 B2 25.90(8) 2_666 2_666 ?
O14 Ba3 B2 111.38(9) 2_566 2_666 ?
O7 Ba3 B2 64.90(8) 1_545 2_666 ?
B5 Ba3 B2 115.10(10) . 2_666 ?
O15 Ba3 B7 87.21(9) . . ?
O10 Ba3 B7 134.07(9) . . ?
O16 Ba3 B7 25.14(9) . . ?
O8 Ba3 B7 129.61(9) 2_666 . ?
O18 Ba3 B7 124.57(8) 1_556 . ?
O11 Ba3 B7 25.35(9) 2_666 . ?
O5 Ba3 B7 85.29(8) 2_666 . ?
O14 Ba3 B7 70.46(8) 2_566 . ?
O7 Ba3 B7 119.87(9) 1_545 . ?
B5 Ba3 B7 112.57(10) . . ?
B2 Ba3 B7 110.64(10) 2_666 . ?
O3 Ba4 O8 116.13(8) . . ?
O3 Ba4 O4 51.22(7) . . ?
O8 Ba4 O4 65.85(7) . . ?
O3 Ba4 O16 62.76(7) . 2_576 ?
O8 Ba4 O16 139.55(8) . 2_576 ?
O4 Ba4 O16 106.87(8) . 2_576 ?
O3 Ba4 O5 135.42(7) . 2_676 ?
O8 Ba4 O5 88.74(7) . 2_676 ?
O4 Ba4 O5 126.46(7) . 2_676 ?
O16 Ba4 O5 121.22(7) 2_576 2_676 ?
O3 Ba4 O17 71.94(7) . 2_676 ?
O8 Ba4 O17 130.92(7) . 2_676 ?
O4 Ba4 O17 97.20(7) . 2_676 ?
O16 Ba4 O17 88.70(7) 2_576 2_676 ?
O5 Ba4 O17 64.11(7) 2_676 2_676 ?
O3 Ba4 O7 150.63(7) . . ?
O8 Ba4 O7 50.37(7) . . ?
O4 Ba4 O7 113.21(7) . . ?
O16 Ba4 O7 108.74(7) 2_576 . ?
O5 Ba4 O7 73.77(7) 2_676 . ?
O17 Ba4 O7 137.40(7) 2_676 . ?
O3 Ba4 O14 109.60(7) . 2_576 ?
O8 Ba4 O14 103.88(7) . 2_576 ?
O4 Ba4 O14 132.34(7) . 2_576 ?
O16 Ba4 O14 49.72(7) 2_576 2_576 ?
O5 Ba4 O14 98.16(7) 2_676 2_576 ?
O17 Ba4 O14 119.15(7) 2_676 2_576 ?
O7 Ba4 O14 59.63(7) . 2_576 ?
O3 Ba4 B1 26.15(8) . . ?
O8 Ba4 B1 91.94(9) . . ?
O4 Ba4 B1 26.09(8) . . ?
O16 Ba4 B1 87.35(9) 2_576 . ?
O5 Ba4 B1 131.17(8) 2_676 . ?
O17 Ba4 B1 79.54(8) 2_676 . ?
O7 Ba4 B1 137.76(8) . . ?
O14 Ba4 B1 128.70(8) 2_576 . ?
O3 Ba4 O11 102.09(7) . 2_676 ?
O8 Ba4 O11 141.11(7) . 2_676 ?
O4 Ba4 O11 148.30(7) . 2_676 ?
O16 Ba4 O11 64.64(7) 2_576 2_676 ?
O5 Ba4 O11 57.14(7) 2_676 2_676 ?
O17 Ba4 O11 53.83(7) 2_676 2_676 ?
O7 Ba4 O11 98.18(7) . 2_676 ?
O14 Ba4 O11 67.46(6) 2_576 2_676 ?
B1 Ba4 O11 123.76(8) . 2_676 ?
O3 Ba4 O19 76.21(7) . 2_676 ?
O8 Ba4 O19 86.15(7) . 2_676 ?
O4 Ba4 O19 63.38(7) . 2_676 ?
O16 Ba4 O19 127.90(7) 2_576 2_676 ?
O5 Ba4 O19 68.88(7) 2_676 2_676 ?
O17 Ba4 O19 46.99(7) 2_676 2_676 ?
O7 Ba4 O19 122.33(7) . 2_676 ?
O14 Ba4 O19 163.73(7) 2_576 2_676 ?
B1 Ba4 O19 62.47(8) . 2_676 ?
O11 Ba4 O19 96.66(6) 2_676 2_676 ?
O3 Ba4 B8 64.45(9) . 2_676 ?
O8 Ba4 B8 110.07(9) . 2_676 ?
O4 Ba4 B8 73.63(9) . 2_676 ?
O16 Ba4 B8 104.96(9) 2_576 2_676 ?
O5 Ba4 B8 72.58(9) 2_676 2_676 ?
O17 Ba4 B8 25.66(9) 2_676 2_676 ?
O7 Ba4 B8 141.17(9) . 2_676 ?
O14 Ba4 B8 144.37(9) 2_576 2_676 ?
B1 Ba4 B8 61.47(10) . 2_676 ?
O11 Ba4 B8 79.24(8) 2_676 2_676 ?
O19 Ba4 B8 24.01(9) 2_676 2_676 ?
O4 Sc1 O15 178.89(10) . . ?
O4 Sc1 O10 89.39(10) . 2_666 ?
O15 Sc1 O10 90.30(10) . 2_666 ?
O4 Sc1 O3 89.74(10) . 2_576 ?
O15 Sc1 O3 90.57(10) . 2_576 ?
O10 Sc1 O3 179.07(9) 2_666 2_576 ?
O4 Sc1 O8 91.77(10) . . ?
O15 Sc1 O8 89.30(10) . . ?
O10 Sc1 O8 89.37(10) 2_666 . ?
O3 Sc1 O8 90.31(10) 2_576 . ?
O4 Sc1 O16 91.17(10) . . ?
O15 Sc1 O16 87.79(10) . . ?
O10 Sc1 O16 94.82(10) 2_666 . ?
O3 Sc1 O16 85.55(10) 2_576 . ?
O8 Sc1 O16 174.91(10) . . ?
O4 Sc1 Ba4 63.63(8) . 2_576 ?
O15 Sc1 Ba4 115.88(8) . 2_576 ?
O10 Sc1 Ba4 132.00(7) 2_666 2_576 ?
O3 Sc1 Ba4 47.76(7) 2_576 2_576 ?
O8 Sc1 Ba4 127.69(7) . 2_576 ?
O16 Sc1 Ba4 50.54(7) . 2_576 ?
O4 Sc1 Ba3 112.94(8) . 2_666 ?
O15 Sc1 Ba3 67.58(8) . 2_666 ?
O10 Sc1 Ba3 48.28(7) 2_666 2_666 ?
O3 Sc1 Ba3 131.88(7) 2_576 2_666 ?
O8 Sc1 Ba3 49.35(7) . 2_666 ?
O16 Sc1 Ba3 132.68(7) . 2_666 ?
Ba4 Sc1 Ba3 176.068(19) 2_576 2_666 ?
O4 Sc1 Ba3 132.60(8) . . ?
O15 Sc1 Ba3 46.30(8) . . ?
O10 Sc1 Ba3 74.34(7) 2_666 . ?
O3 Sc1 Ba3 106.52(7) 2_576 . ?
O8 Sc1 Ba3 131.12(7) . . ?
O16 Sc1 Ba3 47.92(7) . . ?
Ba4 Sc1 Ba3 94.854(16) 2_576 . ?
Ba3 Sc1 Ba3 88.953(13) 2_666 . ?
O4 Sc1 Ba4 47.33(8) . . ?
O15 Sc1 Ba4 133.78(8) . . ?
O10 Sc1 Ba4 99.78(7) 2_666 . ?
O3 Sc1 Ba4 79.37(7) 2_576 . ?
O8 Sc1 Ba4 46.34(7) . . ?
O16 Sc1 Ba4 135.24(7) . . ?
Ba4 Sc1 Ba4 90.062(13) 2_576 . ?
Ba3 Sc1 Ba4 86.078(14) 2_666 . ?
Ba3 Sc1 Ba4 173.983(19) . . ?
O4 Sc1 Ba1 130.39(7) . 1_556 ?
O15 Sc1 Ba1 50.30(7) . 1_556 ?
O10 Sc1 Ba1 135.29(7) 2_666 1_556 ?
O3 Sc1 Ba1 45.36(7) 2_576 1_556 ?
O8 Sc1 Ba1 72.38(7) . 1_556 ?
O16 Sc1 Ba1 102.57(7) . 1_556 ?
Ba4 Sc1 Ba1 89.153(14) 2_576 1_556 ?
Ba3 Sc1 Ba1 92.003(14) 2_666 1_556 ?
Ba3 Sc1 Ba1 87.410(13) . 1_556 ?
Ba4 Sc1 Ba1 96.145(14) . 1_556 ?
O4 Sc1 Ba2 49.47(7) . 1_554 ?
O15 Sc1 Ba2 129.93(7) . 1_554 ?
O10 Sc1 Ba2 42.65(7) 2_666 1_554 ?
O3 Sc1 Ba2 136.64(7) 2_576 1_554 ?
O8 Sc1 Ba2 103.17(7) . 1_554 ?
O16 Sc1 Ba2 81.90(7) . 1_554 ?
Ba4 Sc1 Ba2 94.293(14) 2_576 1_554 ?
Ba3 Sc1 Ba2 84.368(13) 2_666 1_554 ?
Ba3 Sc1 Ba2 95.193(14) . 1_554 ?
Ba4 Sc1 Ba2 80.955(13) . 1_554 ?
Ba1 Sc1 Ba2 175.48(2) 1_556 1_554 ?
O12 Sc2 O9 92.43(10) . . ?
O12 Sc2 O1 85.72(10) . 2_666 ?
O9 Sc2 O1 88.83(10) . 2_666 ?
O12 Sc2 O17 172.93(10) . . ?
O9 Sc2 O17 93.16(10) . . ?
O1 Sc2 O17 90.06(10) 2_666 . ?
O12 Sc2 O11 94.75(10) . . ?
O9 Sc2 O11 172.70(11) . . ?
O1 Sc2 O11 93.06(10) 2_666 . ?
O17 Sc2 O11 79.79(10) . . ?
O12 Sc2 O5 93.56(10) . . ?
O9 Sc2 O5 94.02(9) . . ?
O1 Sc2 O5 177.10(10) 2_666 . ?
O17 Sc2 O5 90.37(10) . . ?
O11 Sc2 O5 84.19(9) . . ?
O12 Sc2 Li3 129.64(18) . 1_656 ?
O9 Sc2 Li3 131.66(18) . 1_656 ?
O1 Sc2 Li3 74.21(19) 2_666 1_656 ?
O17 Sc2 Li3 43.45(18) . 1_656 ?
O11 Sc2 Li3 42.73(17) . 1_656 ?
O5 Sc2 Li3 104.22(19) . 1_656 ?
O12 Sc2 Li1 143.32(13) . 1_656 ?
O9 Sc2 Li1 86.61(15) . 1_656 ?
O1 Sc2 Li1 57.61(13) 2_666 1_656 ?
O17 Sc2 Li1 33.02(13) . 1_656 ?
O11 Sc2 Li1 88.44(15) . 1_656 ?
O5 Sc2 Li1 123.10(13) . 1_656 ?
Li3 Sc2 Li1 45.9(2) 1_656 1_656 ?
O12 Sc2 Ba4 130.56(7) . 2_676 ?
O9 Sc2 Ba4 117.03(7) . 2_676 ?
O1 Sc2 Ba4 130.16(8) 2_666 2_676 ?
O17 Sc2 Ba4 49.61(6) . 2_676 ?
O11 Sc2 Ba4 56.74(7) . 2_676 ?
O5 Sc2 Ba4 48.73(7) . 2_676 ?
Li3 Sc2 Ba4 56.56(17) 1_656 2_676 ?
Li1 Sc2 Ba4 80.84(12) 1_656 2_676 ?
O12 Sc2 Ba3 71.47(7) . 2_666 ?
O9 Sc2 Ba3 134.98(7) . 2_666 ?
O1 Sc2 Ba3 129.54(7) 2_666 2_666 ?
O17 Sc2 Ba3 107.26(7) . 2_666 ?
O11 Sc2 Ba3 47.12(7) . 2_666 ?
O5 Sc2 Ba3 47.64(7) . 2_666 ?
Li3 Sc2 Ba3 86.56(16) 1_656 2_666 ?
Li1 Sc2 Ba3 131.14(13) 1_656 2_666 ?
Ba4 Sc2 Ba3 59.520(10) 2_676 2_666 ?
O12 Sc2 Ba1 45.93(7) . 1_556 ?
O9 Sc2 Ba1 53.79(7) . 1_556 ?
O1 Sc2 Ba1 107.10(8) 2_666 1_556 ?
O17 Sc2 Ba1 141.07(7) . 1_556 ?
O11 Sc2 Ba1 131.87(7) . 1_556 ?
O5 Sc2 Ba1 74.24(7) . 1_556 ?
Li3 Sc2 Ba1 174.55(16) 1_656 1_556 ?
Li1 Sc2 Ba1 139.30(14) 1_656 1_556 ?
Ba4 Sc2 Ba1 122.652(17) 2_676 1_556 ?
Ba3 Sc2 Ba1 88.634(14) 2_666 1_556 ?
O12 Sc2 Ba2 88.16(7) . . ?
O9 Sc2 Ba2 41.70(6) . . ?
O1 Sc2 Ba2 47.14(7) 2_666 . ?
O17 Sc2 Ba2 93.13(7) . . ?
O11 Sc2 Ba2 139.84(7) . . ?
O5 Sc2 Ba2 135.69(7) . . ?
Li3 Sc2 Ba2 108.39(17) 1_656 . ?
Li1 Sc2 Ba2 67.15(13) 1_656 . ?
Ba4 Sc2 Ba2 140.408(19) 2_676 . ?
Ba3 Sc2 Ba2 159.58(2) 2_666 . ?
Ba1 Sc2 Ba2 75.667(12) 1_556 . ?
O6 Sc3 O13 90.66(10) . . ?
O6 Sc3 O2 85.55(11) . 2_576 ?
O13 Sc3 O2 88.78(10) . 2_576 ?
O6 Sc3 O18 174.25(10) . 2_565 ?
O13 Sc3 O18 93.43(10) . 2_565 ?
O2 Sc3 O18 90.50(10) 2_576 2_565 ?
O6 Sc3 O14 94.96(10) . . ?
O13 Sc3 O14 99.30(10) . . ?
O2 Sc3 O14 171.89(10) 2_576 . ?
O18 Sc3 O14 88.37(10) 2_565 . ?
O6 Sc3 O7 97.12(10) . 2_576 ?
O13 Sc3 O7 171.13(11) . 2_576 ?
O2 Sc3 O7 87.60(10) 2_576 2_576 ?
O18 Sc3 O7 78.51(10) 2_565 2_576 ?
O14 Sc3 O7 84.31(9) . 2_576 ?
O6 Sc3 Li2 128.55(19) . 2_576 ?
O13 Sc3 Li2 124.35(18) . 2_576 ?
O2 Sc3 Li2 61.90(17) 2_576 2_576 ?
O18 Sc3 Li2 45.70(18) 2_565 2_576 ?
O14 Sc3 Li2 112.20(17) . 2_576 ?
O7 Sc3 Li2 46.99(17) 2_576 2_576 ?
O6 Sc3 Ba3 131.22(7) . 2_566 ?
O13 Sc3 Ba3 124.25(7) . 2_566 ?
O2 Sc3 Ba3 123.54(8) 2_576 2_566 ?
O18 Sc3 Ba3 48.56(7) 2_565 2_566 ?
O14 Sc3 Ba3 50.83(7) . 2_566 ?
O7 Sc3 Ba3 52.41(6) 2_576 2_566 ?
Li2 Sc3 Ba3 61.65(15) 2_576 2_566 ?
O6 Sc3 Ba4 71.85(7) . 2_576 ?
O13 Sc3 Ba4 139.74(7) . 2_576 ?
O2 Sc3 Ba4 124.17(7) 2_576 2_576 ?
O18 Sc3 Ba4 107.22(7) 2_565 2_576 ?
O14 Sc3 Ba4 48.87(7) . 2_576 ?
O7 Sc3 Ba4 47.86(7) 2_576 2_576 ?
Li2 Sc3 Ba4 93.72(16) 2_576 2_576 ?
Ba3 Sc3 Ba4 59.475(10) 2_566 2_576 ?
O6 Sc3 Ba2 45.94(7) . 1_554 ?
O13 Sc3 Ba2 53.34(7) . 1_554 ?
O2 Sc3 Ba2 108.59(8) 2_576 1_554 ?
O18 Sc3 Ba2 139.67(7) 2_565 1_554 ?
O14 Sc3 Ba2 77.15(7) . 1_554 ?
O7 Sc3 Ba2 135.54(7) 2_576 1_554 ?
Li2 Sc3 Ba2 170.45(16) 2_576 1_554 ?
Ba3 Sc3 Ba2 127.834(17) 2_566 1_554 ?
Ba4 Sc3 Ba2 91.251(15) 2_576 1_554 ?
O6 Sc3 Ba1 85.53(7) . . ?
O13 Sc3 Ba1 40.11(6) . . ?
O2 Sc3 Ba1 48.75(7) 2_576 . ?
O18 Sc3 Ba1 95.00(7) 2_565 . ?
O14 Sc3 Ba1 139.35(7) . . ?
O7 Sc3 Ba1 136.08(7) 2_576 . ?
Li2 Sc3 Ba1 98.36(15) 2_576 . ?
Ba3 Sc3 Ba1 143.238(19) 2_566 . ?
Ba4 Sc3 Ba1 157.20(2) 2_576 . ?
Ba2 Sc3 Ba1 74.324(12) 1_554 . ?
O6 Sc3 Ba1 44.92(7) . 2_575 ?
O13 Sc3 Ba1 101.84(7) . 2_575 ?
O2 Sc3 Ba1 43.41(8) 2_576 2_575 ?
O18 Sc3 Ba1 130.00(7) 2_565 2_575 ?
O14 Sc3 Ba1 134.08(8) . 2_575 ?
O7 Sc3 Ba1 80.96(7) 2_576 2_575 ?
Li2 Sc3 Ba1 88.09(17) 2_576 2_575 ?
Ba3 Sc3 Ba1 133.368(18) 2_566 2_575 ?
Ba4 Sc3 Ba1 90.962(14) 2_576 2_575 ?
Ba2 Sc3 Ba1 83.665(14) 1_554 2_575 ?
Ba1 Sc3 Ba1 70.301(12) . 2_575 ?
B4 O1 Sc2 145.4(2) . 2_666 ?
B4 O1 Ba2 98.4(2) . 1_554 ?
Sc2 O1 Ba2 105.46(10) 2_666 1_554 ?
B4 O1 Ba2 94.4(2) . 2_666 ?
Sc2 O1 Ba2 101.19(9) 2_666 2_666 ?
Ba2 O1 Ba2 108.46(8) 1_554 2_666 ?
B3 O2 Sc3 151.1(3) . 2_576 ?
B3 O2 Li2 79.7(3) . . ?
Sc3 O2 Li2 73.19(18) 2_576 . ?
B3 O2 Ba1 97.2(2) . 1_556 ?
Sc3 O2 Ba1 106.01(10) 2_576 1_556 ?
Li2 O2 Ba1 123.3(2) . 1_556 ?
B3 O2 Ba1 91.7(2) . 2_576 ?
Sc3 O2 Ba1 99.78(9) 2_576 2_576 ?
Li2 O2 Ba1 134.2(2) . 2_576 ?
Ba1 O2 Ba1 102.31(9) 1_556 2_576 ?
B1 O3 Sc1 125.9(2) . 2_576 ?
B1 O3 Ba4 93.8(2) . . ?
Sc1 O3 Ba4 97.38(9) 2_576 . ?
B1 O3 Ba1 98.6(2) . 2_575 ?
Sc1 O3 Ba1 101.44(9) 2_576 2_575 ?
Ba4 O3 Ba1 144.99(10) . 2_575 ?
B1 O4 Sc1 164.1(2) . . ?
B1 O4 Ba4 90.6(2) . . ?
Sc1 O4 Ba4 100.04(10) . . ?
B1 O4 Ba2 85.98(19) . 1_554 ?
Sc1 O4 Ba2 99.24(9) . 1_554 ?
Ba4 O4 Ba2 117.68(9) . 1_554 ?
B1 O4 Ba4 82.10(19) . 2_576 ?
Sc1 O4 Ba4 82.44(8) . 2_576 ?
Ba4 O4 Ba4 118.07(8) . 2_576 ?
Ba2 O4 Ba4 122.91(9) 1_554 2_576 ?
B2 O5 Sc2 144.8(2) . . ?
B2 O5 Li2 79.5(3) . . ?
Sc2 O5 Li2 103.72(19) . . ?
B2 O5 Ba4 118.4(2) . 2_676 ?
Sc2 O5 Ba4 96.61(9) . 2_676 ?
Li2 O5 Ba4 81.63(19) . 2_676 ?
B2 O5 Ba3 89.98(19) . 2_666 ?
Sc2 O5 Ba3 98.60(9) . 2_666 ?
Li2 O5 Ba3 153.95(19) . 2_666 ?
Ba4 O5 Ba3 82.63(6) 2_676 2_666 ?
B1 O6 Sc3 140.9(2) . . ?
B1 O6 Ba2 91.80(19) . 1_554 ?
Sc3 O6 Ba2 103.09(9) . 1_554 ?
B1 O6 Ba1 91.09(19) . 2_575 ?
Sc3 O6 Ba1 105.20(10) . 2_575 ?
Ba2 O6 Ba1 130.41(9) 1_554 2_575 ?
B2 O7 Li2 100.7(3) . . ?
B2 O7 Sc3 125.5(2) . 2_576 ?
Li2 O7 Sc3 83.9(2) . 2_576 ?
B2 O7 Ba4 90.7(2) . . ?
Li2 O7 Ba4 164.5(2) . . ?
Sc3 O7 Ba4 98.22(9) 2_576 . ?
B2 O7 Ba3 142.5(2) . 1_565 ?
Li2 O7 Ba3 84.4(2) . 1_565 ?
Sc3 O7 Ba3 91.90(8) 2_576 1_565 ?
Ba4 O7 Ba3 80.16(6) . 1_565 ?
B2 O8 Sc1 150.8(2) . . ?
B2 O8 Ba4 96.7(2) . . ?
Sc1 O8 Ba4 99.25(9) . . ?
B2 O8 Ba3 92.20(19) . 2_666 ?
Sc1 O8 Ba3 95.14(9) . 2_666 ?
Ba4 O8 Ba3 131.95(10) . 2_666 ?
B3 O9 Sc2 136.1(2) . . ?
B3 O9 Ba2 113.8(2) . . ?
Sc2 O9 Ba2 107.69(9) . . ?
B3 O9 Ba1 86.4(2) . 1_556 ?
Sc2 O9 Ba1 93.33(9) . 1_556 ?
Ba2 O9 Ba1 108.99(8) . 1_556 ?
B5 O10 Sc1 135.9(2) . 2_666 ?
B5 O10 Ba2 96.8(2) . 2_667 ?
Sc1 O10 Ba2 106.24(10) 2_666 2_667 ?
B5 O10 Ba3 92.2(2) . . ?
Sc1 O10 Ba3 97.26(9) 2_666 . ?
Ba2 O10 Ba3 134.57(10) 2_667 . ?
B7 O11 Li3 96.3(3) 2_666 1_656 ?
B7 O11 Sc2 136.1(2) 2_666 . ?
Li3 O11 Sc2 92.8(3) 1_656 . ?
B7 O11 Ba3 93.9(2) 2_666 2_666 ?
Li3 O11 Ba3 149.7(3) 1_656 2_666 ?
Sc2 O11 Ba3 99.48(9) . 2_666 ?
B7 O11 Ba4 135.2(2) 2_666 2_676 ?
Li3 O11 Ba4 75.0(3) 1_656 2_676 ?
Sc2 O11 Ba4 88.61(8) . 2_676 ?
Ba3 O11 Ba4 77.78(6) 2_666 2_676 ?
B5 O12 Sc2 140.8(2) . . ?
B5 O12 Ba1 94.4(2) . 1_556 ?
Sc2 O12 Ba1 102.43(10) . 1_556 ?
B5 O12 Ba2 89.51(19) . 2_667 ?
Sc2 O12 Ba2 104.09(9) . 2_667 ?
Ba1 O12 Ba2 132.07(9) 1_556 2_667 ?
B4 O13 Sc3 135.1(2) . . ?
B4 O13 Ba1 111.1(2) . . ?
Sc3 O13 Ba1 110.84(10) . . ?
B4 O13 Ba2 87.2(2) . 1_554 ?
Sc3 O13 Ba2 94.70(9) . 1_554 ?
Ba1 O13 Ba2 107.88(8) . 1_554 ?
B7 O14 Sc3 145.7(2) . . ?
B7 O14 Li3 79.8(3) . 2_565 ?
Sc3 O14 Li3 107.3(2) . 2_565 ?
B7 O14 Ba3 119.9(2) . 2_566 ?
Sc3 O14 Ba3 94.24(9) . 2_566 ?
Li3 O14 Ba3 77.7(2) 2_565 2_566 ?
B7 O14 Ba4 90.9(2) . 2_576 ?
Sc3 O14 Ba4 97.80(9) . 2_576 ?
Li3 O14 Ba4 147.7(2) 2_565 2_576 ?
Ba3 O14 Ba4 80.42(6) 2_566 2_576 ?
B5 O15 Sc1 152.8(2) . . ?
B5 O15 Ba3 93.3(2) . . ?
Sc1 O15 Ba3 100.75(10) . . ?
B5 O15 Ba1 90.78(19) . 1_556 ?
Sc1 O15 Ba1 96.55(9) . 1_556 ?
Ba3 O15 Ba1 132.36(10) . 1_556 ?
B7 O16 Sc1 134.8(2) . . ?
B7 O16 Li3 115.6(3) . 1_556 ?
Sc1 O16 Li3 109.5(2) . 1_556 ?
B7 O16 Ba3 95.8(2) . . ?
Sc1 O16 Ba3 97.34(9) . . ?
Li3 O16 Ba3 77.11(18) 1_556 . ?
B7 O16 Ba4 95.6(2) . 2_576 ?
Sc1 O16 Ba4 93.43(9) . 2_576 ?
Li3 O16 Ba4 73.90(18) 1_556 2_576 ?
Ba3 O16 Ba4 150.98(11) . 2_576 ?
B8 O17 Li3 139.6(4) . 1_656 ?
B8 O17 Li1 88.1(3) . 1_656 ?
Li3 O17 Li1 76.8(3) 1_656 1_656 ?
B8 O17 Sc2 128.0(2) . . ?
Li3 O17 Sc2 92.2(3) 1_656 . ?
Li1 O17 Sc2 113.5(2) 1_656 . ?
B8 O17 Ba4 90.33(19) . 2_676 ?
Li3 O17 Ba4 81.0(3) 1_656 2_676 ?
Li1 O17 Ba4 143.3(2) 1_656 2_676 ?
Sc2 O17 Ba4 96.09(9) . 2_676 ?
B6 O18 Li2 138.6(3) . 1_544 ?
B6 O18 Sc3 130.4(2) . 2_565 ?
Li2 O18 Sc3 86.3(3) 1_544 2_565 ?
B6 O18 Ba3 102.3(2) . 1_554 ?
Li2 O18 Ba3 89.1(2) 1_544 1_554 ?
Sc3 O18 Ba3 96.87(9) 2_565 1_554 ?
B8 O19 Li2 131.9(4) . . ?
B8 O19 Ba2 116.8(2) . 2_677 ?
Li2 O19 Ba2 110.9(3) . 2_677 ?
B8 O19 Ba4 80.4(2) . 2_676 ?
Li2 O19 Ba4 86.4(3) . 2_676 ?
Ba2 O19 Ba4 113.36(9) 2_677 2_676 ?
B6 O20 Li1 134.6(3) . . ?
B6 O20 Li3 123.9(3) . . ?
Li1 O20 Li3 82.2(3) . . ?
B6 O20 Ba1 111.0(2) . . ?
Li1 O20 Ba1 87.8(2) . . ?
Li3 O20 Ba1 110.9(3) . . ?
B3 O21 B8 138.1(3) . 2_677 ?
B3 O21 Li1 124.7(3) . 2_576 ?
B8 O21 Li1 91.4(3) 2_677 2_576 ?
B3 O21 Ba1 88.4(2) . 2_576 ?
B8 O21 Ba1 120.0(2) 2_677 2_576 ?
Li1 O21 Ba1 81.9(2) 2_576 2_576 ?
B4 O22 B6 137.1(3) . . ?
B4 O22 Li1 100.1(3) . 2_565 ?
B6 O22 Li1 96.4(3) . 2_565 ?
B4 O22 Ba2 87.8(2) . 2_666 ?
B6 O22 Ba2 124.5(2) . 2_666 ?
Li1 O22 Ba2 106.8(2) 2_565 2_666 ?
O6 B1 O4 120.3(3) . . ?
O6 B1 O3 120.1(3) . . ?
O4 B1 O3 119.6(3) . . ?
O6 B1 Ba4 158.2(2) . . ?
O4 B1 Ba4 63.27(18) . . ?
O3 B1 Ba4 60.06(18) . . ?
O6 B1 Ba2 63.13(17) . 1_554 ?
O4 B1 Ba2 68.71(18) . 1_554 ?
O3 B1 Ba2 142.8(2) . 1_554 ?
Ba4 B1 Ba2 102.92(11) . 1_554 ?
O6 B1 Ba1 64.02(17) . 2_575 ?
O4 B1 Ba1 170.4(2) . 2_575 ?
O3 B1 Ba1 56.44(16) . 2_575 ?
Ba4 B1 Ba1 109.31(11) . 2_575 ?
Ba2 B1 Ba1 108.83(10) 1_554 2_575 ?
O6 B1 Ba4 94.8(2) . 2_576 ?
O4 B1 Ba4 74.17(18) . 2_576 ?
O3 B1 Ba4 103.1(2) . 2_576 ?
Ba4 B1 Ba4 106.51(10) . 2_576 ?
Ba2 B1 Ba4 113.74(11) 1_554 2_576 ?
Ba1 B1 Ba4 114.77(11) 2_575 2_576 ?
O8 B2 O7 120.0(3) . . ?
O8 B2 O5 120.6(3) . . ?
O7 B2 O5 119.3(3) . . ?
O8 B2 Li2 168.8(3) . . ?
O7 B2 Li2 49.3(2) . . ?
O5 B2 Li2 70.4(2) . . ?
O8 B2 Ba3 61.94(17) . 2_666 ?
O7 B2 Ba3 152.5(2) . 2_666 ?
O5 B2 Ba3 64.11(17) . 2_666 ?
Li2 B2 Ba3 128.9(2) . 2_666 ?
O8 B2 Ba4 58.02(17) . . ?
O7 B2 Ba4 63.81(18) . . ?
O5 B2 Ba4 162.8(2) . . ?
Li2 B2 Ba4 112.4(2) . . ?
Ba3 B2 Ba4 104.97(11) 2_666 . ?
O9 B3 O2 123.3(3) . . ?
O9 B3 O21 123.6(3) . . ?
O2 B3 O21 113.1(3) . . ?
O9 B3 Li2 104.5(3) . . ?
O2 B3 Li2 71.0(3) . . ?
O21 B3 Li2 95.4(3) . . ?
O9 B3 Ba1 69.6(2) . 1_556 ?
O2 B3 Ba1 58.68(19) . 1_556 ?
O21 B3 Ba1 151.8(2) . 1_556 ?
Li2 B3 Ba1 105.4(2) . 1_556 ?
O9 B3 Ba1 136.2(2) . 2_576 ?
O2 B3 Ba1 64.42(19) . 2_576 ?
O21 B3 Ba1 66.59(18) . 2_576 ?
Li2 B3 Ba1 117.4(2) . 2_576 ?
Ba1 B3 Ba1 86.80(10) 1_556 2_576 ?
O9 B3 Ba2 45.55(16) . . ?
O2 B3 Ba2 143.0(3) . . ?
O21 B3 Ba2 87.14(19) . . ?
Li2 B3 Ba2 140.4(2) . . ?
Ba1 B3 Ba2 88.62(9) 1_556 . ?
Ba1 B3 Ba2 99.90(10) 2_576 . ?
O13 B4 O1 122.7(3) . . ?
O13 B4 O22 123.2(3) . . ?
O1 B4 O22 114.0(3) . . ?
O13 B4 Li1 130.0(3) . 2_565 ?
O1 B4 Li1 89.5(3) . 2_565 ?
O22 B4 Li1 48.4(2) . 2_565 ?
O13 B4 Ba2 140.8(2) . 2_666 ?
O1 B4 Ba2 61.46(18) . 2_666 ?
O22 B4 Ba2 66.94(18) . 2_666 ?
Li1 B4 Ba2 86.4(2) 2_565 2_666 ?
O13 B4 Ba2 69.1(2) . 1_554 ?
O1 B4 Ba2 57.84(18) . 1_554 ?
O22 B4 Ba2 154.5(2) . 1_554 ?
Li1 B4 Ba2 144.2(2) 2_565 1_554 ?
Ba2 B4 Ba2 89.59(10) 2_666 1_554 ?
O13 B4 Ba1 47.61(16) . . ?
O1 B4 Ba1 140.3(2) . . ?
O22 B4 Ba1 86.85(19) . . ?
Li1 B4 Ba1 127.2(2) 2_565 . ?
Ba2 B4 Ba1 101.77(10) 2_666 . ?
Ba2 B4 Ba1 88.48(9) 1_554 . ?
O15 B5 O12 120.3(3) . . ?
O15 B5 O10 119.5(3) . . ?
O12 B5 O10 120.1(3) . . ?
O15 B5 Ba3 60.93(18) . . ?
O12 B5 Ba3 159.5(2) . . ?
O10 B5 Ba3 61.69(18) . . ?
O15 B5 Ba2 158.9(2) . 2_667 ?
O12 B5 Ba2 65.30(17) . 2_667 ?
O10 B5 Ba2 57.97(17) . 2_667 ?
Ba3 B5 Ba2 106.24(11) . 2_667 ?
O15 B5 Ba1 64.23(18) . 1_556 ?
O12 B5 Ba1 60.60(17) . 1_556 ?
O10 B5 Ba1 155.7(2) . 1_556 ?
Ba3 B5 Ba1 108.71(12) . 1_556 ?
Ba2 B5 Ba1 109.04(11) 2_667 1_556 ?
O15 B5 Ba3 82.84(19) . 2_666 ?
O12 B5 Ba3 94.2(2) . 2_666 ?
O10 B5 Ba3 95.8(2) . 2_666 ?
Ba3 B5 Ba3 106.08(10) . 2_666 ?
Ba2 B5 Ba3 117.92(12) 2_667 2_666 ?
Ba1 B5 Ba3 108.51(10) 1_556 2_666 ?
O20 B6 O18 125.6(3) . . ?
O20 B6 O22 123.9(3) . . ?
O18 B6 O22 110.5(3) . . ?
O20 B6 Li1 135.1(3) . 2_565 ?
O18 B6 Li1 81.1(3) . 2_565 ?
O22 B6 Li1 50.3(2) . 2_565 ?
O20 B6 Ba3 90.4(2) . 1_554 ?
O18 B6 Ba3 54.34(17) . 1_554 ?
O22 B6 Ba3 124.4(2) . 1_554 ?
Li1 B6 Ba3 131.6(2) 2_565 1_554 ?
O14 B7 O16 121.9(3) . . ?
O14 B7 O11 118.8(3) . 2_666 ?
O16 B7 O11 119.3(3) . 2_666 ?
O14 B7 Li3 68.8(3) . 2_565 ?
O16 B7 Li3 161.3(3) . 2_565 ?
O11 B7 Li3 51.8(2) 2_666 2_565 ?
O14 B7 Ba3 169.6(2) . . ?
O16 B7 Ba3 59.09(17) . . ?
O11 B7 Ba3 60.79(17) 2_666 . ?
Li3 B7 Ba3 107.5(2) 2_565 . ?
O14 B7 Ba4 63.98(18) . 2_576 ?
O16 B7 Ba4 59.42(17) . 2_576 ?
O11 B7 Ba4 164.5(2) 2_666 2_576 ?
Li3 B7 Ba4 123.9(2) 2_565 2_576 ?
Ba3 B7 Ba4 113.46(12) . 2_576 ?
O19 B8 O17 126.1(3) . . ?
O19 B8 O21 124.7(3) . 2_677 ?
O17 B8 O21 109.1(3) . 2_677 ?
O19 B8 Li1 171.5(3) . 1_656 ?
O17 B8 Li1 57.9(3) . 1_656 ?
O21 B8 Li1 52.8(2) 2_677 1_656 ?
O19 B8 Ba4 75.6(2) . 2_676 ?
O17 B8 Ba4 64.01(17) . 2_676 ?
O21 B8 Ba4 133.3(2) 2_677 2_676 ?
Li1 B8 Ba4 112.2(2) 1_656 2_676 ?
O21 Li1 O20 116.3(4) 2_576 . ?
O21 Li1 O22 142.6(5) 2_576 2_565 ?
O20 Li1 O22 99.2(3) . 2_565 ?
O21 Li1 O17 69.0(2) 2_576 1_454 ?
O20 Li1 O17 98.0(4) . 1_454 ?
O22 Li1 O17 119.7(4) 2_565 1_454 ?
O21 Li1 B8 35.75(16) 2_576 1_454 ?
O20 Li1 B8 115.7(4) . 1_454 ?
O22 Li1 B8 136.0(4) 2_565 1_454 ?
O17 Li1 B8 34.02(15) 1_454 1_454 ?
O21 Li1 Li3 105.5(4) 2_576 . ?
O20 Li1 Li3 49.1(3) . . ?
O22 Li1 Li3 106.8(4) 2_565 . ?
O17 Li1 Li3 51.5(3) 1_454 . ?
B8 Li1 Li3 80.2(3) 1_454 . ?
O21 Li1 B6 129.7(4) 2_576 2_565 ?
O20 Li1 B6 90.0(3) . 2_565 ?
O22 Li1 B6 33.26(16) 2_565 2_565 ?
O17 Li1 B6 153.0(4) 1_454 2_565 ?
B8 Li1 B6 153.9(4) 1_454 2_565 ?
Li3 Li1 B6 123.2(3) . 2_565 ?
O21 Li1 B4 153.9(4) 2_576 2_565 ?
O20 Li1 B4 85.0(3) . 2_565 ?
O22 Li1 B4 31.51(15) 2_565 2_565 ?
O17 Li1 B4 94.4(3) 1_454 2_565 ?
B8 Li1 B4 122.8(3) 1_454 2_565 ?
Li3 Li1 B4 76.2(3) . 2_565 ?
B6 Li1 B4 60.49(19) 2_565 2_565 ?
O21 Li1 Li2 69.3(3) 2_576 2_576 ?
O20 Li1 Li2 140.8(4) . 2_576 ?
O22 Li1 Li2 75.8(3) 2_565 2_576 ?
O17 Li1 Li2 118.6(3) 1_454 2_576 ?
B8 Li1 Li2 91.2(3) 1_454 2_576 ?
Li3 Li1 Li2 169.9(3) . 2_576 ?
B6 Li1 Li2 64.2(2) 2_565 2_576 ?
B4 Li1 Li2 104.5(3) 2_565 2_576 ?
O21 Li1 Ba1 63.3(2) 2_576 . ?
O20 Li1 Ba1 57.0(2) . . ?
O22 Li1 Ba1 139.3(3) 2_565 . ?
O17 Li1 Ba1 97.5(3) 1_454 . ?
B8 Li1 Ba1 84.1(2) 1_454 . ?
Li3 Li1 Ba1 82.8(3) . . ?
B6 Li1 Ba1 108.4(2) 2_565 . ?
B4 Li1 Ba1 141.3(3) 2_565 . ?
Li2 Li1 Ba1 101.7(3) 2_576 . ?
O21 Li1 Sc2 95.9(3) 2_576 1_454 ?
O20 Li1 Sc2 104.2(3) . 1_454 ?
O22 Li1 Sc2 86.2(3) 2_565 1_454 ?
O17 Li1 Sc2 33.53(15) 1_454 1_454 ?
B8 Li1 Sc2 60.81(18) 1_454 1_454 ?
Li3 Li1 Sc2 57.1(2) . 1_454 ?
B6 Li1 Sc2 119.4(3) 2_565 1_454 ?
B4 Li1 Sc2 62.61(18) 2_565 1_454 ?
Li2 Li1 Sc2 114.1(3) 2_576 1_454 ?
Ba1 Li1 Sc2 128.9(2) . 1_454 ?
O21 Li1 Ba2 104.4(3) 2_576 1_454 ?
O20 Li1 Ba2 138.3(3) . 1_454 ?
O22 Li1 Ba2 45.07(18) 2_565 1_454 ?
O17 Li1 Ba2 87.6(2) 1_454 1_454 ?
B8 Li1 Ba2 91.5(2) 1_454 1_454 ?
Li3 Li1 Ba2 112.5(3) . 1_454 ?
B6 Li1 Ba2 69.77(18) 2_565 1_454 ?
B4 Li1 Ba2 53.30(16) 2_565 1_454 ?
Li2 Li1 Ba2 62.12(19) 2_576 1_454 ?
Ba1 Li1 Ba2 163.2(2) . 1_454 ?
Sc2 Li1 Ba2 60.80(12) 1_454 1_454 ?
O19 Li2 O18 123.2(5) . 1_566 ?
O19 Li2 O7 151.1(5) . . ?
O18 Li2 O7 81.9(3) 1_566 . ?
O19 Li2 O5 96.3(3) . . ?
O18 Li2 O5 140.5(4) 1_566 . ?
O7 Li2 O5 59.9(2) . . ?
O19 Li2 O2 119.0(3) . . ?
O18 Li2 O2 78.9(3) 1_566 . ?
O7 Li2 O2 76.6(3) . . ?
O5 Li2 O2 82.2(3) . . ?
O19 Li2 B2 125.5(4) . . ?
O18 Li2 B2 110.9(3) 1_566 . ?
O7 Li2 B2 30.03(16) . . ?
O5 Li2 B2 30.06(13) . . ?
O2 Li2 B2 75.5(2) . . ?
O19 Li2 B3 90.0(3) . . ?
O18 Li2 B3 98.0(3) 1_566 . ?
O7 Li2 B3 101.0(3) . . ?
O5 Li2 B3 80.8(3) . . ?
O2 Li2 B3 29.27(13) . . ?
B2 Li2 B3 88.9(3) . . ?
O19 Li2 Sc3 158.4(4) . 2_576 ?
O18 Li2 Sc3 48.00(18) 1_566 2_576 ?
O7 Li2 Sc3 49.13(17) . 2_576 ?
O5 Li2 Sc3 95.1(3) . 2_576 ?
O2 Li2 Sc3 44.91(14) . 2_576 ?
B2 Li2 Sc3 69.5(2) . 2_576 ?
B3 Li2 Sc3 73.8(2) . 2_576 ?
O19 Li2 Li1 82.6(3) . 2_576 ?
O18 Li2 Li1 56.2(2) 1_566 2_576 ?
O7 Li2 Li1 125.9(3) . 2_576 ?
O5 Li2 Li1 139.5(3) . 2_576 ?
O2 Li2 Li1 63.9(2) . 2_576 ?
B2 Li2 Li1 138.9(3) . 2_576 ?
B3 Li2 Li1 58.8(2) . 2_576 ?
Sc3 Li2 Li1 76.8(2) 2_576 2_576 ?
O19 Li2 Ba3 122.0(4) . 1_565 ?
O18 Li2 Ba3 54.50(18) 1_566 1_565 ?
O7 Li2 Ba3 58.30(18) . 1_565 ?
O5 Li2 Ba3 106.5(2) . 1_565 ?
O2 Li2 Ba3 116.5(2) . 1_565 ?
B2 Li2 Ba3 83.3(2) . 1_565 ?
B3 Li2 Ba3 145.2(3) . 1_565 ?
Sc3 Li2 Ba3 71.61(16) 2_576 1_565 ?
Li1 Li2 Ba3 108.2(2) 2_576 1_565 ?
O19 Li2 Ba4 61.5(2) . 2_676 ?
O18 Li2 Ba4 145.2(3) 1_566 2_676 ?
O7 Li2 Ba4 89.8(3) . 2_676 ?
O5 Li2 Ba4 51.98(15) . 2_676 ?
O2 Li2 Ba4 132.0(3) . 2_676 ?
B2 Li2 Ba4 70.78(19) . 2_676 ?
B3 Li2 Ba4 116.8(3) . 2_676 ?
Sc3 Li2 Ba4 138.6(3) 2_576 2_676 ?
Li1 Li2 Ba4 144.2(3) 2_576 2_676 ?
Ba3 Li2 Ba4 92.54(18) 1_565 2_676 ?
O19 Li2 Ba2 42.1(2) . 2_677 ?
O18 Li2 Ba2 84.4(3) 1_566 2_677 ?
O7 Li2 Ba2 144.8(3) . 2_677 ?
O5 Li2 Ba2 132.8(3) . 2_677 ?
O2 Li2 Ba2 131.9(3) . 2_677 ?
B2 Li2 Ba2 151.9(3) . 2_677 ?
B3 Li2 Ba2 112.9(3) . 2_677 ?
Sc3 Li2 Ba2 131.8(3) 2_576 2_677 ?
Li1 Li2 Ba2 69.2(2) 2_576 2_677 ?
Ba3 Li2 Ba2 87.48(18) 1_565 2_677 ?
Ba4 Li2 Ba2 83.29(16) 2_676 2_677 ?
O20 Li3 O11 157.9(6) . 1_454 ?
O20 Li3 O17 97.8(4) . 1_454 ?
O11 Li3 O17 82.1(3) 1_454 1_454 ?
O20 Li3 O14 106.1(3) . 2_565 ?
O11 Li3 O14 62.7(3) 1_454 2_565 ?
O17 Li3 O14 137.3(5) 1_454 2_565 ?
O20 Li3 Li1 48.8(3) . . ?
O11 Li3 Li1 121.1(4) 1_454 . ?
O17 Li3 Li1 51.7(2) 1_454 . ?
O14 Li3 Li1 127.8(4) 2_565 . ?
O20 Li3 B7 136.6(4) . 2_565 ?
O11 Li3 B7 31.98(17) 1_454 2_565 ?
O17 Li3 B7 112.8(4) 1_454 2_565 ?
O14 Li3 B7 31.36(15) 2_565 2_565 ?
Li1 Li3 B7 136.2(5) . 2_565 ?
O20 Li3 O16 114.6(4) . 1_554 ?
O11 Li3 O16 85.0(3) 1_454 1_554 ?
O17 Li3 O16 114.5(4) 1_454 1_554 ?
O14 Li3 O16 87.2(3) 2_565 1_554 ?
Li1 Li3 O16 142.3(4) . 1_554 ?
B7 Li3 O16 80.6(3) 2_565 1_554 ?
O20 Li3 Sc2 123.1(4) . 1_454 ?
O11 Li3 Sc2 44.49(18) 1_454 1_454 ?
O17 Li3 Sc2 44.31(18) 1_454 1_454 ?
O14 Li3 Sc2 93.1(3) 2_565 1_454 ?
Li1 Li3 Sc2 77.0(3) . 1_454 ?
B7 Li3 Sc2 70.5(2) 2_565 1_454 ?
O16 Li3 Sc2 119.5(3) 1_554 1_454 ?
O20 Li3 Ba4 131.3(4) . 2_575 ?
O11 Li3 Ba4 67.6(2) 1_454 2_575 ?
O17 Li3 Ba4 60.0(2) 1_454 2_575 ?
O14 Li3 Ba4 119.5(3) 2_565 2_575 ?
Li1 Li3 Ba4 106.3(3) . 2_575 ?
B7 Li3 Ba4 91.4(2) 2_565 2_575 ?
O16 Li3 Ba4 55.73(18) 1_554 2_575 ?
Sc2 Li3 Ba4 72.73(16) 1_454 2_575 ?
O20 Li3 Ba3 81.0(3) . 1_554 ?
O11 Li3 Ba3 104.8(3) 1_454 1_554 ?
O17 Li3 Ba3 164.6(5) 1_454 1_554 ?
O14 Li3 Ba3 56.64(17) 2_565 1_554 ?
Li1 Li3 Ba3 129.7(3) . 1_554 ?
B7 Li3 Ba3 76.9(2) 2_565 1_554 ?
O16 Li3 Ba3 53.70(17) 1_554 1_554 ?
Sc2 Li3 Ba3 147.4(3) 1_454 1_554 ?
Ba4 Li3 Ba3 109.4(3) 2_575 1_554 ?
O20 Li3 Ba1 41.7(2) . . ?
O11 Li3 Ba1 156.8(3) 1_454 . ?
O17 Li3 Ba1 81.0(3) 1_454 . ?
O14 Li3 Ba1 138.9(3) 2_565 . ?
Li1 Li3 Ba1 57.4(2) . . ?
B7 Li3 Ba1 164.7(3) 2_565 . ?
O16 Li3 Ba1 87.7(3) 1_554 . ?
Sc2 Li3 Ba1 124.4(2) 1_454 . ?
Ba4 Li3 Ba1 90.1(2) 2_575 . ?
Ba3 Li3 Ba1 88.2(2) 1_554 . ?

_refine_diff_density_max         0.642
_refine_diff_density_min         -1.053
_refine_diff_density_rms         0.179

